N A N O E X P R E S S
Synthesis and Properties of the La
O. V. Chukova1*
, S. G. Nedilko1
, A. A. Slepets2
, S. A. Nedilko2
and T. A. Voitenko2
The La1−xCaxVO4and La1−x−yEuyCaxVO4(0≤x,y≤0.2) micro/nanosized powders were prepared by aqueous nitrate–
citrate sol–gel synthesis. Phase composition of the sample depends on thexandyvalues. The La0.9Ca0.1VO4is crystallized
in monoclinic structure up to thex= 0.1. The La0.9Eu0.05Ca0.05VO4sample was also attributed to the monoclinic structure.
Increasing concentration of europium and calcium ions in La1−x−yEuyCaxVO4solid solutions leads to the change of the
crystal structure, and subsequently, stabilization of the tetragonal phase takes place.
The obtained samples were characterized by XRD analysis, SEM microscopy, and IR spectroscopy. Luminescence properties of the synthesized powders were studied. Emission of the La1−xCaxVO4samples is weak and consists of wide
bands in the 450–800 nm spectral range. The observed bands at 570 and 630 were ascribed to electron transitions in the distorted VO43−vanadate groups. Emission of the La1−x−yEuyCaxVO4samples consists of narrow spectral lines in the 550–
730 nm spectral range. The lines are caused by the 5D0→ 7
FJ electron transitions in the Eu 3+
ions. The Ca2+ ions incorporation increases the intensity of the Eu3+ions luminescence. Structure of the spectra depends on Ca2+ concentration and excitation wave length. The carried out analysis has revealed that Eu3+ions form at least two different types of emission centers in the La1−x−yEuyCaxVO4samples. The assumption is made that type I centers are formed by
the Eu3+ions in their regular positions in the crystal lattice, while the type II centers have complex structure and consist of Eu3+ions, Ca2+cations, and oxygen vacancies.
Keywords:Vanadate, Sol–gel, Eu3+, Luminescence
Rare earth orthovanadates are very interesting class of compounds which have very important applications in various fields involving chemistry and biology, luminescent nanoparticles, and light transformers [1–4]. Orthovana-dates can exhibit unusual magnetic, optical, thermally acti-vated, and X-ray luminescence properties . Nanosized orthovanadates have also attracted considerable research interest as perspective photocatalyst systems for photocata-lytic water splitting. The widely used photocatalyst TiO2is
active only under ultraviolet light irradiation [1, 6], while europium (EuVO4)  and lanthanum (LaVO4) 
ortho-vanadates are of a special attention as the most promising visible-light-driven photocatalysts . These compounds are chemically stable and non-toxic [10, 11]. Their range of biological applications includes fluorescent probes for
single-molecule tracking, drug development, protein detec-tion, and fluorescent bio labeling [2, 11, 12].
Actually, some of the abovementioned applications re-quire vanadate materials with improved efficiency of lumi-nescence excitation under light from near UV and violet spectral ranges [4, 13–15]. The search for new vanadate compounds for these needs is carried out using variations of two and more cations in their composition including partial iso- and heterovalent substitutions [16–19]. It was shown previously that intensities of luminescent emission of the RE activators in orthovanadate compounds can be effectively increased with the A2+modifying cations (A = Ca, Sr, Ba, Pb, etc.) [4, 16, 20–22]. Moreover, properties of compositions with such heterovalent substitutions are strongly dependent on concentration ratios of the A2+ cat-ions. Besides, our recent investigations have shown that in-crease of intensity of luminescence emission of rare earth orthovanadates can be also achieved with improvement of method of synthesis and morphology of the nanoparticles [14, 23]. Therefore, we expect that expansion of the best of
1Faculty of Physics, Taras Shevchenko National University of Kyiv, 64/13,
Volodymyrska Str, 01601 Kyiv, Ukraine
Full list of author information is available at the end of the article
our recent practices for synthesis of the rare earth orthova-nadate nanaparticles onto the same compositions with heterovalent substitutions could bring an additional raise of emission intensity of luminescent orthovanadate nano-particles. At the first step in this direction, we use the Ca2+ modifying impurities as the cheapest reagent.
The aim of this work is to study synthesis procedures, structural features, and morphological and optical char-acteristics of the nanosized La1−xCaxVO4 and La1−x− yEuyCaxVO4(0≤x,y≤0.2) compounds. Various methods
can be applied for synthesis of the orthovanadates nano-particles, such as solid state [16, 23], hydrothermal , solution combustion , and sol–gel methods [14, 25]. One of the most promising ways to perform an excellent homogenization for nanoscale sizes of particles, high re-activity of the compounds, and morphology that satisfy enhanced emission intensity is the sol–gel method.
The La1−xCaxVO4 and La1−x−yEuyCaxVO4 samples
(0≤x, y≤0.2) were prepared by aqueous nitrate–citrate sol–gel synthesis route using citric acid (CA) as a com-plexing agent. Lanthanum (III) and europium (III) ni-trates La(NO3)3 (99.0%, High Purity Chemicals),
Eu(NO3)3 (99.0%, High Purity Chemicals), calcium (II)
nitrate Ca(NO3)2 (99.0%, High Purity Chemicals), and
ammonium metavanadate NH4VO3(99.0%, High Purity
Chemicals) were used as starting compounds. They were weighted according to the desired stoichiometric molar ratio. Nitric acid (HNO3), distilled water, and ammonia
(NH3·4H2O) were used as solvents and reagents to
regu-late the pH of the solutions. Firstly, NH4VO3 was
dis-solved in concentrated ammonia solution by stirring at 70–80 °C temperature. Then, the CA dissolved in dis-tilled water with a small amount of NH3·4H2O was
added. Next, La(NO3)3, Eu(NO3)3, and Ca(NO3)2 were
added. To prevent precipitation, the pH that reached the value of ~6–7 was controlled. Finally, the same amount of the aqueous solution of the complexing agent CA was repeatedly added to the reaction mixture to prevent crystallization of metal salts during the gelation process. The clear solution was concentrated by slow evaporation at 80–90 °C in an open beaker. A transparent gel has been formed after evaporation of nearly 90% of the water during the continuous stirring. The powders were ob-tained after drying in an oven at 100 °C. The powders were step by step calcined for 5 h at the range from 150 to 700 °C. Figure 1 illustrates the process of synthesis.
Phase compositions and crystal lattice parameters of the synthesized samples were determined using X-ray diffract-ometer DRON-3M (CuKα-radiation with a Ni filter). The diffraction patterns were taken with a 2°/min step. Characterization of the samples’ morphology was made using scanning electron microscope (SEM) Tescan Mira 3 LMU with 20-nm electronic beam diameter. The second-ary electron detector (InBeam) could be used, if there is a need, to enhance spatial resolution up to 1 nm. Infrared (IR) spectra of the samples were recorded on PerkinElmer IR spectrometer using the KBr pellet method in the 1400– 400 cm−1 range. Luminescence spectra were measured at high resolution equipment using DFS-12 and DMR-23 diffraction spectrometers with excitation by diode lasers, nitrogen gas laser, and xenon lamp (see more de-tails in [26, 27]).
Results and Discussion X-ray Diffraction
The X-ray diffraction (XRD) patterns of the synthesized La1−xCa−VO4 and La1−x−yEuyCaxVO4(x≤0.2, y≤0.2)
samples are shown in Fig. 2. It was found that the La0.9Ca0.1VO4sample is crystallized in monoclinic
struc-ture; a space group is P21/n (see Fig. 2). This result is
well matched with a standard card of monoclinic LaVO4
(JCPDS PDF2 50-0367) (see Fig. 2). The La0.9Eu
0.05-Ca0.05VO4 sample with low concentration of the Ca2+
and Eu3+ impurities is also attributed to the monoclinic structure. Proximity of the Ca2+ (1.12 nm), La3+ (1.16 nm), and Eu3+ (1.066 nm) ions radii provides an opportunity for calcium and europium ions’incorporation into three plus cation’s sites. Besides, we see that small quantities of the Ca2+(x≤0.1) and Eu3+ions (y≤0.05) can enter to the crystal lattice without change of the mono-clinic LaVO4structure.
Increasing concentrations of the Eu3+and Ca2+ impur-ities leads to formation of the monoclinic and tetragonal phase mixture (Fig. 2). The La0.6Eu0.2Ca0.2VO4 sample
becomes related to tetragonal structure, belonging to the I41/amd space group. This result is agreed with the standard card of tetragonal LaVO4 (JCPDS PDF2
32-0504) (see Fig. 2). If some amount of the residual mono-clinic phase is still presented in these samples, it was below the detection limit of our XRD equipment.
Therefore, increasing concentration of europium and calcium ions in La1−x−yEuyCaxVO4(x,y≤0.2) solid
solu-tions leads to the change of the crystal structure, and sub-sequently, stabilization of the tetragonal phase takes place.
Morphology and Chemical Element Analysis
The set of characteristic SEM images of the La1−x−yEu
x-CayVO4 samples are shown in Fig. 3. The top two
im-ages, a and b, show areas of ~5 × 5μm; in other words, general view of samples is given, whereas other images, c–f, show small separated areas, up to ~0.5 × 0.5 μm size. It is easy to see from general view that samples con-sist of grains of different sizes, from tens of nanometers to 1 μm. Grains of large sizes (0.2–1.0 μm) are agglom-erates of smaller ones, and they have no certain shapes. Detailed view of agglomerates and of small grains (Fig. 3c–f ) show that they are formed by nanoparticles of size from 20 to 100 nm. The La0.9Eu0.05Ca0.05VO4
samples with low concentration of the Eu and Ca impur-ities consist of grains of 0.1–0.2 μm-size, those are formed by nanoparticles of 10–20-nm size (Fig. 3c). The nanoparticles of larger size, ~100 nm, are characteristic for the samples with higher concentration of dopants, La0.8Eu0.1Ca0.1VO4. Most of them have polyhedral
shapes with clearly defined edges and angles between them (Fig. 3d). The particles with the observed polyhe-dral shapes have to be assigned to the crystal system of lower symmetry. Thus, most likely, they should be regarded as a manifestation of the monoclinic phase of the studied samples. The next increase of the Eu3+ and Ca2+ dopant concentrations also generates particles of ~100-nm sizes (Fig. 3e). Despite of the poor quality of this image, it is possible to conclude that the shapes of the particles are closer to the cylinders and rods.The same shapes are observed for the samples of the highest dopant concentration, La0.6Eu0.2Ca0.2VO4(Fig. 3f ).
How-ever, it should be noted that size of the particles is smaller for these samples; it is preferably 30–60 nm.
Thus, we can say that the change of the powder sam-ples’composition is accompanied by the changes in the size and morphology of their constituent particles. These changes are consistent with the XRD data on the struc-ture and phase composition of the samples. Therefore, the SEM data can be interpreted as indicating that the samples of higher dopant concentration are mixtures of monoclinic and tetragonal phases and the content of the latter increases when the content of europium and cal-cium ions increases.
Chemical element analysis was performed for 3–5 various agglomerates or grains for each sample using SEM tools. Monitoring area from which information about content of atoms have been taken was larger than e-beam size, and it was near (30–40) × (30–40)μm. We have found that La, Eu, Ca, V, and O are the main
Fig. 2X-ray diffraction patterns of the La1−xCaxVO4and La1−x−
components of the samples. In certain cases, some quan-tity of carbon atoms revealed that obvious occurred when edge zone of grains or grains of small thickness were monitored. (Powder samples were fixed on special carbon-covered scotch tape for SEM measurements.) Average data are accumulated in Table 1.
Analysis of data presented in Table 1 gives possibility to note the next.
1. Data of the SEM experiments on the contents of the La3+ions in the synthesized samples (first column of the Table1) are quite closed to the expected compositions (see the far right column of the Table1).
2. If we take the total content of the Eu3+and Ca2+
ions, it is easy to see that the experimentally measured data are quite close to the expected
compositions. However, it is easy to see that the predicted simultaneous fourfold increase of ions Eu3+ and Ca2+content (from 0.05 up to 0.20 at.%) is not implemented for the actual synthesized samples. We can observe when the content of the Eu3+ions increases by ~10 times, the content of the Ca2+ions
Fig. 3The SEM images of the La0.8Ca0.2VO4 (a), La0.6 Eu0.2Ca0.2VO4 (b,f), La0.9 Eu0.05Ca0.05VO4 (c), La0.8 Eu0.1Ca0.1VO4 (d), and La0.7 Eu0.15Ca0.15VO4 (e) samples
Table 1Calculated starting composition of the La, Ca, and Eu atoms in the samples under synthesis, average content of atoms (in at.%), and evaluated composition of the synthesized samples
Starting composition La Eu Ca Evaluated composition La0.8Ca0.2 41.2 – 9.4 La0.81Ca0.19
La0.9Eu0.05Ca0.05 26.60 0.73 1.76 La0.92Eu0.02Ca0.06
La0.8Eu0.10Ca0.10 20.81 2.34 1.11 La0.86Eu0.10Ca0.04
La0.7Eu0.15Ca0.15 12.30 3.30 1.73 La0.71Eu0.19Ca0.10
increases only by ~2–3 times. This is due both to specific of the samples (heterogeneity of sizes, shapes, and thickness of grains of powder, etc.) and features of the method (a significant error for light elements, the effect of electron beam on oxide surfaces, etc.). Nevertheless, this result should be taken into account when describing other properties of the synthesized compounds. First of all, it concerns their luminescent properties. To avoid misunderstanding, we will not
change following designation of samples noted in the “Synthesis”
IR spectroscopy study of the La1−xCaxVO4and La1−x− yEuyCaxVO4 (0≤x, y≤0.2) samples was performed to
confirm their structure and composition. The view of the IR spectra in the range of 400–1100 cm−1
(Fig. 4) is typical for the LaVO4 IR absorption spectra previously
measured in this range [28–30]. These spectra are also very similar to the IR spectra of other lanthanide orthova-nadates LnVO4 (Ln = Y, Ce−Yb) [28, 31], multi-metal
orthovanadates such as M3Ln(XO4)2and M2M′Ln(XO4)2
(M, M′= Na, K, Rb)  and vanadates of the M′′3V2O8
(M′′= Mg, Ca, Sr, Ba, and Zn) type [33–35]. Namely, the spectra are similar to all of compounds; those lattices are built by isolated tetrahedral VO43−molecular groups.
It is well known that the bending (ν2 and ν4) and stretching vibrations (ν1 and ν3) of O–V–O bonds of the VO43− anion form IR absorption spectra of various
orthovanadates in the range 400–700 and 700–1100 cm−1
, respectively [36, 37]. In fact, measured by us, spectrum of the undoped LaVO4 contains separated weak bands
lo-cated in the range 400–700 cm−1
, while stronger wide band lies in the range 700–1100 cm−1
(Fig. 4, curve 1). Sharp peak at 434 cm−1and blurred band centered near 550 cm−1compose IR spectra of this sample in the former range. The main peak at ~778 cm−1and three strongly overlapped other ones located at ~820, 850, and 880 cm−1 form wide band (Fig. 4, curve 1). (All the mentioned peaks are marked by arrows close to the curve 1 in Fig. 4, and their positions are in Table 2).
When LaVO4is doped by the Ca2+ions, the shapes of
spectral bands and peaks positions are changed, but these changes are not as striking as one could expect, but we should note that composition of peaks changes. As a result, six peaks marked by arrows can be found on the curves 2 and 3 of Fig. 4 in the range of wide absorp-tion band.
Fig. 4IR absorption spectra of the LaVO4 (1), La0.9Ca0.1VO4 (2), La0.8Ca0.2VO4 (3), La0.8Eu0.1Ca0.1VO4 (4), and La0.6Eu0.2Ca0.2VO4 (5)
Table 2IR peaks positions (in cm−1) and their attributions to vibration modes in the VO4
LaVO4 La0.9Ca0.1VO4 La0.8Ca0.2VO4 La0.8Eu0.1Ca0.1VO4 La0.6Eu0.2Ca0.2VO4 Vibration modes
434 438 436 439 440 ν4
570 553 553
778 780 777 783 780
802 801 802 801
820 822 824 821 820
850 836; 850 835; 850 835; 854 836; 852
880 874 875 875 874 ν1
If the Eu3+ ions are added to the La1−xCaxVO4
com-pounds, then band of stretching vibrations becomes more complicated and its components are more overlapped (Fig. 4, curves 4 and 5). Thus, six or seven peaks can be distinguished there (see arrows), and shape and structure of the band become very similar to ones previously pub-lished on IR absorption spectra of the LaVO4containing
Eu3+ions [31, 36]. (The peaks positions of all measured IR absorption bands are accumulated in Table 2.)
The exact assignment of spectral components to a cer-tain type of modes is difficult, especially that concerns stretching vibration range. Due to the low Cs symmetry
of the VO43− molecular anion in monoclinic LaVO4, four
IR lines lying close to each other can appear in this range of spectra. Our experimental findings are in good agreement with noted above theoretical prediction. Mentioned fact causes strong overlapping of the lines, that is why they are revealed as one complex wide band. Doping with calcium ions causes a distortion of certain amount of vanadates groups. As a result, additional peaks appear in the spectrum. Besides, as we have shown above, all co-doped samples under our study are a mix-ture of monoclinic and tetragonal LaVO4 phases and
contribution of the phases depends on the dopant con-centration. The VO43− molecular groups possess D2d
symmetry in tetragonal LaVO4. So, two lines of Eu and
A2usymmetry can be found in the range of stretching
vi-brations if morphology of the VO43− groups corresponds
to ideal tetragonal lattice structure. Really, neighbor en-vironment and symmetry of some VO43− groups in
tet-ragonal lattice are also deformed by Ca2+ ions, and all of VO43− internal vibrations can occur in the IR spectra.
As previously have been reported, the calculated  and measured  peak positions of the IR absorption lines for tetragonal LaVO4are close to those for
mono-clinic LaVO4. Thus, the eight lines can form the range of
stretching vibrations, we suppose. Change of the phase composition leads to mentioned changes of the shape of the IR bands and their positions. Regarding published theoretical and experimental data, a possible assignment of all measured features was made (Table 2). Additional studies are necessary in order to clarify the origin of the bands that are in the ranges 500–700 and 900–1000 cm−1
. We can only note that similar features were previously observed in the IR absorption spectra of some Ca contain-ing orthovanadates [33, 34].
In any cases, we are able to state that observed IR spectra confirm that anionic sub-lattice of studied vana-dates is built by VO43−molecular anions.
Emission of the La1−xCaxVO4 samples is observed in a
wide spectral range from 400 to 800 nm. The observed bands are complex. The photoluminescence (PL) spectra
contain two wide and strongly overlapped components at position of their maximum near ~570 and ~630 nm (Fig. 5). The band positions and structure of the spectra are similar to those described previously as for undoped nanosized LaVO4 and Ba3V2O8 compounds, as well as
for activated Sr2.91V2O8:0.06Eu3+, Ca2NaMg2V3O12:Eu3+,
and Na2LnMg2V3O12vanadate phosphors [17, 21, 39, 40].
The observed bands can be assigned to electron transi-tions in the VO43−groups; those are constituents of
men-tioned compounds. The charge transfer transitions of 3d orbitals electron of the V5+ion to the 2p orbital electron of the O2−ion inside of the VO43−groups are the nature of
this luminescence [40, 41]. According to energy scheme of the vanadate tetrahedron, emission bands at 570 and 630 nm are connected respectively with 3T2 and 3T1→ 1
A1 electron transitions in the VO43− groups [39–41].
These transitions are forbidden in the ideal Tdsymmetry
of the VO43− group. Distortion of the VO43−tetrahedrons
from the ideal symmetry in the crystal lattice of LaVO4
enhances the spin–orbit interaction and makes these tran-sitions partially allowed . As we noted above, in the monoclinic phase of the La1−xCaxVO4samples, the VO43−
groups have distorted symmetry. Besides, some of these groups are affected by Ca2+ions. The VO43− group also is
of lower symmetry than Td in tetragonal La1−x−yEu
y-CaxVO4samples. Thus, we have all the reasons to assign
the observed 570 and 630 nm bands to the 3T2 and 3
T1→1A1electron transitions in the VO43−groups.
Emission of the La1−x−yEuyCaxVO4 samples is
ob-served in the 550–730 nm spectral range and consists of narrow spectral lines, and undoubtedly, they are caused by radiation transitions in Eu3+ions (Figs. 6 and 7). The emission intensity increases if content of dopants in-creases in the range (0≤x≤0.15) (Fig. 7).
Excitation spectra of all the synthesized samples are typical for luminescence excitation spectra of undoped and doped with Eu3+ions LaVO4[20–23, 42–44]. They
contain wide band with peak position at about 320 nm (Fig. 8). Also, two narrow weak peaks at ~405 and ~475 nm are presented in the spectra of the Eu-containing samples.
Structure of the emission spectra depends on the exci-tation wave length,λex(Fig. 6), and on the concentration of the Ca2+and Eu3+dopants (Fig. 7). For the La0.8Eu0.
1-Ca0.1VO4sample, which is just a mixture of monoclinic
and tetragonal phases (see Fig. 2), the PL lines at 586, 592.5, 607, 611, 614, 618, 649, 697, and 702 nm (marked by arrows at Fig. 6, curve 2) are observed at all applied
λex. (We call this set of the lines as first set.) Note also that the ratio of intensity of the lines at 611, 614, and 618 nm changes if λex varies. Besides, intensive lines at 580, 590, 591.7, 595.6, 608.7, and 622 and lines near 645, 651, 655, 706, and 708 nm (marked by arrows with as-terisk at Fig. 6, curve 3, and at Fig. 7, curve 4) are dis-tinctively observed in the spectra measured at λex= 405 nm. (We call this set of the lines as second set.) So, the measured emission spectra are the superposition of two sets of luminescence lines. Since we have shown above that the sample La0.8Eu0.1Ca0.1VO4 is just a
mix-ture of two crystalline phases, we have first to suppose
Fig. 6Emission spectra of the La0.8Eu0.1Ca0.1VO4 (1–4) and La0.9Eu0.1VO4 (5) samples atλex = 532 (1,5), 473 (2), 405 (3), and 337 nm (4)
Fig. 7Emission spectra of the La1−x−yEuyCaxVO4(1–4) and La1−
xEuxVO4(5) samples atλex= 405 nm;x,y= 0.05 (1), 0.1 (2,5), 0.15 (3), 0.2 (4)
that these sets are related with emission of Eu3+centers in monoclinic and tetragonal phases.
With the intent to clarify this assumption, we performed study of the luminescence spectra dependence on the samples composition at the same excitation wave length,
λex= 405 nm (Fig. 7). We found that the emission spectra of the samples where x= 0.1 and 0.15 are very close to each other (Fig. 7, curves 3 and 4). This finding agrees with the statement that these samples are the mixture of two phases. Tetragonal phase dominates in the La0.6Eu
0.2-Ca0.2VO4sample, and we see thatsecond set of the
lumi-nescence lines also dominates in the spectrum of this
sample, but we see also that mentioned before line at 618 nm is vanished in this spectrum (Fig. 7, curve 4). When observe the emission spectrum of the La0.9Eu
0.05-Ca0.05VO4 (Fig. 7, curve 1), we see that first set of lines
mainly reveals in the spectrum (Fig. 7, curve 1). As the La0.9Eu0.05Ca0.05VO4sample is monoclinic (see Fig. 2), we
should relate thefirst setof lines to emission of Eu3+ions in monoclinic crystal phase. At the same time, we note that line at 618 nm is also vanished in this spectrum. So, we concluded that not only competition between content of the crystal phases influence luminescence behavior. Let us discuss the question in detail.
The observed narrow PL lines are caused by the5D0→ 7
FJ (J = 0, 1, 2, 3, 4) electron radiation transitions in the
inner4fnshell of the Eu3+ions. The7FJenergy levels may
be split in the crystal field on the 2j + 1 sub-levels, but some of possible transitions can be forbidden by the sym-metry rules . If the Eu3+ ions occupy the site of the La3+ ions in tetragonal LaVO4 crystal lattice (I41/amd
space group), they have D2dsite symmetry. In such a case,
group theory predicts no luminescence peaks from5D0→ 7
F0 transition, two lines from the 5D0→7F1 and three
lines from the5D0→7F2transitions. If the Eu3+ions
oc-cupy the site of the La3+ions in monoclinic LaVO4crystal
lattice (P21/n space group), they have C1site symmetry. In
this case, group theory predicts manifestation all of pos-sible transitions: one luminescence peak from the5D0→ 7
F0 transition, three lines from 5D0→7F1 and five lines
from the5D0→7F2transitions .
So, it was not surprising that accounting the spectra in Fig. 6 in sum, we have found one line for the 5D0→7F0
(spectral range 570–585 nm), five lines (586, 592.5, 590, 591.7, 595.6 nm) for the 5D0→7F1(spectral range 585–
600 nm), and seven lines (607, 614, 618, 608.7, 611, 614, 622 nm) for 5D0→7F2 transitions (spectral range 600–
650 nm), as this figure shows the luminescence spectra of the sample which is mixture of the monoclinic and tetrag-onal phases. This statement also concerns the spectra 2 and 3 in Fig. 7, as they also represent luminescence of the mixture, x= 0.1 and 0.15, respectively. It was surprising that we see intensive line from the 5D0→7F0 transition
for the La0.6Eu0.2Ca0.2VO4sample which represents only
tetragonal crystal structure (Fig. 7, curve 4). Moreover, we see that the spectrum of the monoclinic La0.9Eu
0.05-Ca0.05VO4 sample (Fig. 7, curve 1) is lesser complicated
than it might be expected to this structure. At the same time, it is important that luminescence intensity of these samples is lower if compared to intensity for other sam-ples shown in this Figure. As we go from spectrum 1 to spectrum 4 in Fig. 7, the contribution of monoclinic phase decreases. These results mean that other factors, not only crystal structure, significantly determine luminescence be-havior of the samples under study. Thus, we supposed that as shown in Figs. 6 and 7, curves 2–4, spectral trans-formations are mainly related to luminescence behavior of tetragonal phase, especially to role of Ca2+cations, as their concentration increases by 2–3 times when gone fromx= 0.1 to 0.2 (see the “Morphology and Chemical Element analysis”section).
In fact, obtained results mean that at least two of dif-ferent type luminescence centers formed by the ions Eu3
in the sample of tetragonal structure contribute to the PL spectra. We ascribed the abovementioned spectral lines to emission of type I (“first set”of lines) and type II of the centers (“second set”of lines). Emission line from the 5D0→7F0 transition (580 nm) is observed only for
the type II centers, and the most intensive lines of the
D0→7F2 and 5D0→7F4 transitions for these centers
are located at 622 and 708 nm, respectively. For type I centers, the most intensive lines are located at 614 and 697 nm. These spectral features allow us to do assump-tion that types I and II of centers are characterized by different symmetry of the Eu3+ ions environment: the type I centers are characterized by higher site symmetry and the type II centers are characterized by lower site symmetry in the crystal lattices . We supposed that type I centers are formed by the Eu3+ions in their regu-lar positions in the crystal lattice (D2dsymmetry).
As for the type II centers, we suppose that they can be formed by Eu3+ions disturbed by defects generated as a result of Ca2+ cations incorporation into LaVO4crystal
lattice. To confirm this supposition, we performed addi-tive experimental study of the sample that does not con-tain Ca2+ ions, namely, La0.9Eu0.1VO4 composition of
tetragonal structure [14, 23] (Figs. 6 and 7, curves 5). Taking into account that above noted lines of type II centers (e.g., lines at 622 and 708 nm) were not observed for the Ca2+-free sample (Fig. 7, curve 5), we concluded that the most possible origin of the type II centers is the Eu3+ ions disturbed by Ca-induced defects. In the case of the doped with calcium LaVO4lattice, the Ca2+
replacements. Thus, for the Ca2+ dopants arrangement in the LaVO4crystal lattice, we should expect that some
of the Eu3+ ions are under the effect of both neighbor Ca2+cations and oxygen vacancy. Thus, we can assume that such Eu3+ ions are just the type II of the lumines-cence centers, and their local symmetry is lower if com-paring to symmetry of the type I centers. Taking into account that 5D0→7F0 transition emission line (near
580 nm) is observed in the spectra (Figs. 6 and 7), the symmetry of type II centers may be C2 or Cs [44, 45].
The C2 symmetry of the Eu3+ surrounding in the I41/
amd space group of orthovanadates can be achieved only by equal distortions of two oxygen positions. Therefore, we assume that case of the Cssymmetry of the Eu3+
sur-rounding at the type II centers is more probable.
Excitation spectra measured in the emission lines corre-sponded to different types of centers (614 and 622 nm for types I and II centers, respectively) confirmed made above description, as these spectra revealed some differences (Fig. 8). The wide band at 320 nm is more intensive in the excitation spectra of type I centers. The 320-nm band is also observed in the spectra of the La0.9Eu0.1VO4sample
(Fig. 8, curve 2). This band is caused by electron transi-tions in the vanadate VO43− groups. Therefore, the type I
centers are better excited through the matrix than type II centers, that confirms our assumptions about relation of the type I centers with the Eu3+ions in the regular posi-tions in the crystal lattice.
Total emission intensity of the La1−x−yEuyCaxVO4
sam-ples have shown essential increasing when dopant concen-tration increases up tox,y= 0.15 (Fig. 9, curve 1). Similar dependence reveal peak intensity of the 614 and 622 nm lines caused by luminescence of types I and II centers, re-spectively (Fig. 9, curve 2 and 3), but we see that main contribution to luminescence enhance is related with emission of type II of centers. Therefore, spectral behavior of the type II luminescence centers is not only single
manifestation of the Ca2+cations influence on the La1−x−
yEuyCaxVO4emission. The Ca2+doping enhances also
ef-ficiency of this type of luminescence centers.
As for quenching of the luminescence intensity at x, y> 0.15, it should be noted that several mechanisms may be responsible for this. First, it is concentration quench-ing related with Eu3+content. Then, as we described in the “Morphology and Chemical Element Analysis” sec-tion, the sizes of particle decreases for the La0.6Eu
0.2-Ca0.2VO4 sample. So, the surface quenching can be
important mechanism in this case.
Surely, made assumption about role of the Ca2+ ions in luminescence of the lanthanum vanadate, LaVO4,
co-doped with Eu3+and Ca2+ions requires additional study, and we plan to carry out it in the future.
The La1−xCaxVO4 and La1−x−yEuyCaxVO4 (0≤x, y≤
0.2) micro/nanosized powders were prepared by aqueous nitrate–citrate sol–gel synthesis. Phase composition of the sample depends on thexandyvalues.
The La0.9Ca0.1VO4 is crystallized in monoclinic
struc-ture up to thex= 0.1.
The La0.9Eu0.05Ca0.05VO4 sample was also attributed
to the monoclinic structure.
Increasing concentration of europium, Eu3+, and cal-cium ions, Ca2+, in La1−x−yEuyCaxVO4 solid solutions
leads to the change of the crystal structure, and subse-quently, stabilization of the tetragonal phase takes place.
Phase transformation and especially Ca2+ ions influ-ence IR spectroscopy and luminescinflu-ence behavior of studied compounds, as Ca2+ ions impact both on VO43−
molecular groups and La3+and Eu3+ions.
Emission of the La1−xCaxVO4samples consists of wide
bands in the 450–800 nm spectral range. These bands were ascribed to electron transitions in the distorted VO43−
Emission of the La1−x−yEuyCaxVO4 samples is
ob-served in the 550–730 nm spectral range, and it consists of narrow spectral lines. These lines are caused by the
D0→7FJelectron transitions in the Eu3+ions. The Eu3+
ions form two types of emission centers in the samples under study. The assumption was made that type I cen-ters are formed by the Eu3+ ions in their regular posi-tions in the crystal lattice, while the type II centers have complex structure and they consists of Eu3+ ions, Ca2+ cations, and oxygen vacancies.
IR:Infrared; PL: Photoluminescence; RE: Rare earth; SEM: Scanning electron microscopy; XRD: X-ray diffraction
The authors thank the leaders and people of the“NanoMedTech LLC”company (Kyiv, Ukraine), who provided modern SEM equipment for the study samples, for their help during the study. Authors are grateful to Leading Engineer Iryna
Nedielko (Taras Shevchenko National University of Kyiv) for her help in the XRD measurements.
Publication is based on the research provided by the grant support of the State Fund for Fundamental Research (project F64/44-2016).
SN contributed to the development of strategy of the work and its scientific management, luminescent SEM study, and processing and discussion of the measurement results. OCh contributed to the luminescent spectra measurements, processing and analysis of taken results, and discussion of luminescence and IR spectroscopy results. SAN contributed to the development of strategy of the chemical part of this work and its scientific management, synthesis adjustment, and analysis of IR spectroscopy and XRD results. AS contributed to the solution for synthesis and samples’preparation, IR spectroscopy measurement and processing of measurement results, XRD study, and processing and analysis of their results. TV contributed to the study, analysis, and discussion of the synthesis results, IR spectroscopy and XRD study, and discussion of the measurement results. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
1Faculty of Physics, Taras Shevchenko National University of Kyiv, 64/13,
Volodymyrska Str, 01601 Kyiv, Ukraine.2Faculty of Chemistry, Taras
Shevchenko National University of Kyiv, 64/13, Volodymyrska Str, 01601 Kyiv, Ukraine.
Received: 29 December 2016 Accepted: 27 April 2017
1. Li W, Li D, Lin Y, Wang P, Chen W, Fu X, Shao Y (2012) Evidence for the active species involved in the photodegradation process of methyl orange on TiO2. J Phys Chem 116(5):3552–3560
2. Shen J, Sun L-D, Yan C-H (2008) Luminescent rare earth nanomaterials for bioprobe applications. Dalton Trans 42(14):5661–5808
3. Huse M, Norby T, Haugsrudz R (2011) Proton conductivity in acceptor-doped LaVO4. J Electrochem Soc 158(8):B857–B865
4. Lin H-Y, Chang W-F, Chu S-Y (2013) Luminescence of (Ca, Sr)3(VO4)2:Pr3+, Eu3 + phosphor for use in CuPc-based solar cells and white light-emitting diodes. J Lumin 133:194–199
5. Zhang Y, Li G, Yang X, Yang H, Lu Z, Chen R (2013) Monoclinic BiVO4 micro-/nanostructures: microwave and ultrasonic wave combined synthesis and their visible-light photocatalytic activities. J Alloys Compd 551:544–550 6. Wang D, Li R, Zhu J, Shi J, Han J, Zong X, Li C (2012) Photocatalytic water
oxidation on BiVO4with the electrocatalyst as an oxidation cocatalyst: essential relations between electrocatalyst and photocatalyst. J Phys Chem 116(8):5082–5089
7. Garg AB, Errandonea D (2015) High-pressure powder X-ray diffraction study of EuVO4. J Solid State Chem 226:147–153
8. Cheng X, Guo D, Feng S, Yang K, Wang Y, Ren Y, Song Y (2015) Structure and stability of monazite- and zircon-type LaVO4under hydrostatic pressure. Opt Mater 49:32–38
9. Tamilmani V, Sreeram KJ, Nair BU (2015) Catechin assisted phase and shape selection for luminescent LaVO4zircon. RSC Adv 5(100):82513–82523 10. Mialon G, Gohin M, Gacoin T, Boilot J-P (2008) High temperature strategy
for oxide nanoparticle synthesis. ACS Nano 2(12):2505–2512
11. Venkataraman BV, Sudha S (2005) Vanadium Toxicity. Asian J Exp Sci 19(2):127–134 12. Clark AS, Fagant JM, Mitch WE (1985) Selectivity of the insulin-like actions of vanadate on glucose and protein metabolism in skeletal muscle. Biochem J 232:273–276
13. Tyminski A, Grzyb T, Lis S (2016) REVO4-based nanomaterials (RE = Y, La, Gd, and Lu) as hosts for Yb3+/Ho3+, Yb3+/Er3+, and Yb3+/Tm3+ions: structural and up-conversion luminescence studies J Am Ceram Soc (Article in Press)
14. Chornii V, Chukova O, Nedilko SG, Nedilko SA, Voitenko T (2016) Enhancement of emission intensity of LaVO4:RE3+luminescent solar light absorbers. Phys Status Solidi C 13(1):40–46
15. Nedilko SG, Chornii V, Chukova O, Degoda V, Bychkov K, Terebilenko K, Slobodyanik M (2016) Luminescence properties of the new complex La, BiVO4: Mo, Eu compounds as materials for down-shifting of VUV–UV radiation. Radiat Meas 90:282–286
16. Qin C, Huang Y, Seo H (2013) Structure and luminescence of new red-emitting materials-Eu3+-doped triple orthovanadates NaALa(VO4)2(A = Ca, Sr, Ba). J Am Ceram Soc 96:1181–1187
17. Yoon SJ, Park K (2014) Synthesis and photoluminescent properties of white-emitting Sr2.91V2O8:0.06Eu3+phosphors. Op Mater 36:1305–1310
18. Ardanova LI, Chukova OV, Getman EI, Marchenko VI, Nedilko SG, Scherbatskyi VP (2002) Luminescent properties of the Ca5(VO4)3OH apatites with the heterovalence calcium replacement on alkali and rare-earth elements. Funct Mater 9(2):326–331
19. Chukova O, Nedilko S, Moroz Z, Pashkovskyi M (2003) Luminescence of the samarium ions doped in the complex oxides with heterovalence substitution. J Lumin 102–103:498–503
20. Shinde KN, Singh R, Dhoble SJ (2014) Photoluminescent characteristics of the single-host white-light-emitting Sr3-3x/2(VO4)2:xEu (0 < x < 0.3) phosphors for LEDs. J Lumin 146:91–96
21. Park KC, Mho S (2007) Photoluminescence properties of Ba3V2O8, Ba3(1−x)Eu2xV2O8 and Ba2Y2/3V2O8:Eu3+. J Lumin 122–123:95–98
22. Tian L, Mho S (2007) Enhanced photoluminescence of YVO4:Eu3+by codoping the Sr2+, Ba2+or Pb2+ion. J Lumin 122–123:99–103
23. Chukova O, Nedilko SA, Nedilko SG, Sherbatsky V, Voitenko T (2013) Comparable structural and luminescent characterization of the La1-xEuxVO4 solid solutions synthesized by solid state and co-precipitation methods. Solid State Phenom 200:186–192
24. Xu Z, Li C, Hou Z, Peng C, Lin J (2011) Morphological control and luminescence properties of lanthanide orthovanadate LnVO 4 (Ln = La to Lu) nano-/microcrystals via hydrothermal process. Cryst Eng Comm 13:474–482 25. Chumha N, Kittiwachana S, Thongtem T, Thongtem S, Kaowphong S (2014)
Synthesis and characterization of GdVO4nanostructures by a tartaric acid-assisted sol–gel method. Ceram Int 40:16337–16342
26. Boyko R, Chukova OV, Gomenyuk OV, Nagornyi PG, Nedilko SG (2005) Origin of red luminescence of sodium titanium phosphate crystals contained chromium and titanium ions. Phys Stat Sol 2(1):712–715
27. Chukova O, Nedilko S, Scherbatskyi V (2010) Luminescent spectroscopy and structure of centers of the impurity Eu3+ions in lead tungstate crystals. J Lumin 130(10):1805–1812
28. Liu J, Li Y (2007) Synthesis and self-assembly of luminescent Ln3+-doped LaVO4uniform nanocrystals. Adv Mater 19:1118–1122
29. Liu G, Duan X, Li H, Dong H (2009) Hydrothermal synthesis, characterization and optical properties of novel fishbone-like LaVO4:Eu3+nanocrystals. Mater Chem Phys 115:165–171
30. Von Escobar ME, Baran EJ (1978) Uber die tetragonale Modifikation von Lanthan-orthowanadat. Z Anorg Allg Chem 441:273–277
31. Fang ZM, Hong Q, Zhou ZH, Dai SJ, Weng WZ, Wan HL (1999) Oxidative dehydrogenation of propane over a series of low-temperature rare earth orthovanadate catalysts prepared by the nitrate method. Catalysis Letters 61:39–44 32. Rghioui L, Benarafa L, El Jastimi J, El Hajji A, Lorriaux A, Wallart F (2012)
Vibrational spectra and force field studies of K1,125Rb1,875La(VO4)2vanadate. J Mater Environ Sci 3(1):58–65
33. Baran EJ (1976) Die Schwingungsspektren von Ca3(VO4)2und Ca,(AsO,). Z Anorg Allg Chem 497:131–136
34. Parhi P, Manivannan V, Kohl S, McCurdy P (2008) Synthesis and characterization of M3V2O8(M = Ca, Sr and Ba) by a solid-state metathesis approach. Bull Mater Sci (India) 31(6):885–890
35. Siebert H (1954) Kraftkonstante und Strukturchemie. V Struktur der Sauerstoffsäuren Z Anorg Allg Chem 275:225–240
36. Nakamoto K (1963) Infrared spectra of inorganic and coordination compounds. Wiley, New York, p 410
37. Melvin L (1974) Symmetry principles in solid state and molecular physics. Wiley, New York, p 499
38. Sun L, Zhao X, Li Y, Li P, Sun H, Cheng X, Fan W (2010) First-principles studies of electronic, optical and vibrational properties of LaVO4polymorph. J Appl Phys 108(9):093519–10
39. Sobszyk M, Szymański D (2013) A study of optical properties of Sm3+ions in
40. Chukova O, Nedilko SA, Nedilko SG, Voitenko T, Gomenyuk O, Sheludko V (2015) Study of temperature behavior of luminescence emission of LaVO4 and La1-xEuxVO4powders. Solid State Phenom 230:153–159
41. Song D, Guo C, Li T (2015) Luminescence of the self-activated vanadate phosphors Na2LnMg2V3O12(Ln = Y, Gd). Ceram Int 41:6518–6524 42. Setlur AA, Comanzo HA, Srivatava AM, Beers WWJ (2005) Spectroscopic
evaluation of a white light phosphor for UV-LEDs-Ca2NaMg2V3O12:Eu3+. J Electrochem Soc 152(12):H205–H208
43. Tao ZX, Tsuboi TJ, Huang YL, Huang W, Cai PQ, Seo HJ (2014)
Photoluminescence properties of Eu3+-doped glaserite-type orthovanadates CsK2Gd(VO4)2. Inorg Chem 53(8):4161–4168
44. Park SW, Yang HK, Chung JW, Chen Y, Moon BK, Cho BC, Jeon JH, Kim JH (2010) Photoluminescent properties of LaVO4Eu3+by structural transformation. Physica B 405:4040–44
45. Wybourne BG (1965) Spectroscopic properties of ions in crystals. Wiley, New York, p 236
Submit your manuscript to a
journal and beneﬁ t from:
7 Convenient online submission
7 Rigorous peer review
7 Immediate publication on acceptance
7 Open access: articles freely available online
7 High visibility within the ﬁ eld
7 Retaining the copyright to your article